### Hierarchical simulations of hybrid polymer

### –

### solid

### materials

Karen Johnstonaand Vagelis Harmandaris*abc

Complex polymer–solid materials have gained a lot of attention during the last 2–3 decades due to the fundamental physical problems and the broad spectrum of technological applications in which they are involved. Therefore, signiﬁcant progress concerning the simulations of such hybrid soft–hard nanostructured systems has been made in the last few years. Simulation techniques vary from quantum to microscopic (atomistic) up to mesoscopic (coarse-grained) level. Here we give a short overview of simulation approaches on model polymer–solid interfacial systems for all diﬀerent levels of description. In addition, we also present a brief outlook concerning the open questions in thisﬁeld, from the point of view of both physical problems and computational methodologies.

### 1

### Introduction

Hybrid materials, which contain so–hard matter interfaces, are becoming increasingly important in devices, such as solar cells, fuel cells, biosensors,etc.The properties of such devices should be tuned to provide optimal performance, and nanopatterning, such as nanoparticle arrays or nanopores, is a promising

technique. The behaviour of somatter close to an interface can diﬀer drastically from its bulk behaviour and since these systems typically have a high interface density the behaviour of the materials at the nanoscale aﬀects the properties of the system at the macroscale. For example, the strength of polymer adsorption at the interface may govern the properties of the nanostructured material. The key issues that must be addressed in hybrid multi-phase materials are the change in various properties (structural, dynamical, mechanical, electrical,etc.) at the interface compared to the bulk and the extent of these changes from the solid surface, which is of particular importance for nanostructured materials.1–3 The study of hybrid polymer–solid systems is very chal-lenging for both experiment and simulation due to the very

Karen Johnston obtained a PhD with Prof. Tony Paxton from the Department of Physics in Queen's University Belfast, UK in 2003. Her rst postdoctoral position was in Rutgers Univer-sity, New Jersey, USA, where she continued with density func-tional theory calculations of perovskite materials in the group of Prof. Karin Rabe. In 2005, she moved to Prof. Risto Nieminen's group in the Helsinki University of Technology (now Aalto University), Finland and became interested in polymer adhesion. Currently, she is a post-doctoral researcher in the Max Planck Institute for Polymer Research in Mainz, Germany and uses a hierarchical multiscale approach to model polymer–solid interfaces.

Vagelis Harmandaris is an
Assis-tant Professor in the Department
of Applied Mathematics at the
University of Crete, Greece. Before
he was a research associate in
Max Planck Institute for Polymer
Research (Mainz, Germany),
working with Prof. K. Kremer on
multi-scale modelling of polymer
systems. He received his PhD in
chemical engineering from the
University of Patras (Greece) in
2002, under the direction of Prof.
D. Theodorou and V. Mavrantzas on atomistic modelling of polymer
viscoelasticity. His research interests focus on the development of
hierarchical multi-scale simulation approaches and rigorous
math-ematical methods for modelling molecular and biomolecular
complex systems, with particular emphasis on understanding the
structure–property relationships of polymer–solid hybrid materials.
a_{Max Planck Institute for Polymer Research, Ackermannweg 10, Mainz 55128,}

Germany. E-mail: johnston@mpip-mainz.mpg.de

b_{Department of Applied Mathematics, University of Crete, GR-71409 Heraklion, Crete,}

Greece

c_{IACM FORTH GR-71110 Heraklion, Crete, Greece. E-mail: vagelis@tem.uoc.gr}

Cite this:Soft Matter, 2013,9, 6696

Received 31st January 2013 Accepted 13th May 2013

DOI: 10.1039/c3sm50330e

www.rsc.org/softmatter

### REVIEW

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

Creative Commons Attribution-NonCommercial 3.0 Unported Licence.

broad range of length and time scales involved. This is a general
characteristic of all macromolecular systems since there are
diﬀerent characteristic time scales associated with the motion
of various parts (segments) of the chain.4_{However, for hybrid}
multiphase polymer–solid systems the range of length and time
scales may be even broader due to the presence of the
inter-faces. For example, concerning the length scales, the behavior
of the polymer at the interface is related to the interaction of
each atom with the solid surface and typically ranges from
lengths of a few (1–2) A, for strongly (chemically) adsorbed˚
molecules, up to around 1 nm for weakly (physically) adsorbed
molecules that interact with the surfaceviavan der Waals (vdW)
interactions. In contrast, the behaviour of the entire system is
related to the dispersion (i.e.arrangement) of the solid phase
(e.g.nanoparticles) in the polymer matrix, which might involve
macroscopic dimensions of the order of a few mm. Therefore, at
least 7–8 orders of magnitude in length scale are involved in
hybrid multi-phase nanostructured materials. Things are even
more complicated concerning the relevant time scales of hybrid
materials. Atomic bond vibrations (within a molecule or
between atoms in a molecule and atoms of a crystal) are
typi-cally characterized by times of a few fs (1015 s), whereas
conformational changes associated with dihedral transitions
take place in times of the order of a few ps (1012 s) for
temperatures well above the glass transition, Tg, and much
longer times for temperatures close to Tg. Relaxation of the
entire chain can be of the order of seconds even for
tempera-tures far fromTg, whereas the dynamics of various segments
along the chain is characterized by all intermediate time scales.
In addition, the dynamics can be even slower for chains
adsorbed on solid surfaces. Therefore, the dynamical behavior
of collective phenomena related to the dynamics of the polymer
matrix near a solid phase might span more than about 15 orders
of magnitude.

Considering all of the above, various experimental
approaches have been used to study diﬀerent aspects of
poly-mer–solid interfacial systems related to structure,
conforma-tions and dynamics.5–8 _{For experiment, the challenge lies in}
characterization of the structural and dynamical properties
near the interface, which is either too small to be resolved by the
experimental technique or which is masked by the larger bulk
region. For example, many experimental investigations have
focused on the change in the glass transition temperature of
polymer materials close to an interface, with conicting
results.9–12 _{Recently, experimental work has focused on the}
properties near a solid surface; however, the results are
inconclusive.8,12

Furthermore, various experimental methods have been
developed for studying a variety of potential applications of
polymer nanocomposites.13–16 _{For example, the dispersion of}
nanosized particles, or carbon nanotubes, into a polymer matrix
has been shown to alter signicantly the mechanical as well as
rheological, electrical and barrier properties of pure
poly-mers.13,16 _{Clearly, there is a need for techniques probing the}
polymer–solid interfaces at the molecular level.

Simulations can complement experiments by providing the detailed structural, conformational and dynamical properties

near the interface. However, for simulations the diﬃculty lies in treating the wide range of time and length scales simulta-neously. To overcome such problems, diﬀerent approaches have been used to model systems at various levels of descrip-tion. To model the processing of polymeric materials, the traditional approach is to average out the details at the molec-ular level and simulate the system at the continuum level using, for example,uid dynamics ornite-element methods. These methods rely on input parameters, such as viscosity, density and elastic moduli, which are usually assumed to be constant throughout the model system. Obtaining these parameters is a non-trivial issue even for bulk polymer systems. For hybrid polymer–solid systems the application of continuum simula-tions is even more diﬃcult, since properties of the materials at the interface may be very diﬀerent to the bulk properties. In addition, the continuum approximation breaks down at the nanoscale level. This is even more important for interfacial systems, in which the material parameters might vary as a function of distance from the interface.17

In contrast, particle-based simulation methods provide a more detailed description of somatter and can be used to predict various properties, such as density, structure, and dynamics at the molecular level. These particle-based methods can be further subdivided into atomistic and coarse-grained (CG) models. CG models, which represent groups of atoms by single particles, can be used to describe systems in the meso-scopic regime. The choice of CG representation is a crucial factor in all CG simulation approaches, and depends crucially on the physical problem and the questions to be addressed. To obtain a more quantitative comparison between realistic model systems and experimental quantities, atomistic models can be used, which have the advantage of a detailed all-atom repre-sentation of the hybrid material. However, the accuracy of atomistic models depends on the classical force elds and standard classical force elds are usually not designed to describe the interaction with solid surfaces and changes in chemical bonding. Therefore, to understand the chemical bonding of a molecule with a solid surface and to develop accurate force elds one must use quantum mechanical methods.

It is clear from the above discussion that in order to build up an understanding of a complex hybrid multi-phase system and its properties, it is necessary to connect diﬀerent levels of description by using a multiscale modelling approach. Hierar-chical multiscale simulation methodologies are usually described via typical length-time pictures, such as the one shown in Fig. 1. Thegure gives a qualitative picture of the various techniques, with the corresponding length and time scales, as well as representative snapshots from a polymer–solid interfacial system starting from the quantum level, through classical microscopic atomistic models, mesoscopic coarse-grained models and up to continuum methods. Of particular importance is the systematic procedure needed in order to link the diﬀerent levels of description.

The purpose of this review is to discuss the main topics related to the application of modeling and simulation tech-niques to the polymer–solid interfacial system. This is a broad

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

subject that covers diﬀerent systems and simulation method-ologies at various length and time scales. Here we will focus on quantum, microscopic and mesoscopic methods, with partic-ular emphasis on particle-based simulation approaches. For a discussion of the continuum modeling of hybrid multi-phase materials see ref. 1 and 17 and references therein.

We organize the review as follows. In the next section we discuss molecule–surface studies at the quantum level and the development of accurate classical force elds based on quantum data. Atomistic molecular dynamics and Monte Carlo studies of polymer–solid interfaces are presented in Section 3. In Section 4 an overview of the mesoscopic simulation approaches and coarse-graining techniques is presented. Field theoretical approaches are discussed briey in Section 5. Finally, the Outlook discusses open questions related to the physical problems, as well as technical aspects, in modeling so–hard interfaces.

### 2

### Quantum-based interface force

### ﬁ

### eld

### development

As stated in the Introduction, the properties of hybrid materials
are strongly dependent on the surface interaction. To account
properly for the chemical bonding and properties of adsorbed
molecules quantum mechanical calculations are necessary.
Post-Hartree–Fockab initioapproaches, such as Møller–Plesset
perturbation theory or coupled-cluster (CCSD), directly solve the
Schr¨odinger equation and are among the most accurate
quantum mechanical methods available. However, they are
computationally expensive and are limited to small system sizes
of only a few atoms. Density functional theory (DFT) is an
alternative quantum mechanical approach, which is
computa-tionally less expensive than quantum chemistry calculations.
DFT is described in detail in textbooks20_{so this section focuses}
on recent eﬀorts to include van der Waals forces in DFT and
describes various schemes for the development of interface
forceelds based on DFT results.

In DFT, the total energy,E, can be written as a functional of the electronic charge density,r

E[r]¼Ts[r] +EH[r] +Vext[r] +Exc[r]. (1)

Tsis the kinetic energy of a system of non-interacting elec-trons with the same electronic density as the real system,EHis the Hartree energy of the electrons,Vextis the external energy, which in the simplest case is just the Coulomb energy of elec-trons in the potential ofxed nuclei, andExc[r] is the so-called exchange and correlation energy. The last term implicitly includes the diﬀerence in the kinetic energy of the real and

ctitious systems as well as the many-body interactions in the electron–electron interaction energy. The analytical form of the exchange and correlation functional is unknown and it is the approximation of this term that limits the applicability of DFT.

The local density approximation (LDA) was successfully used
for many solid materials where the electron density is fairly
homogeneous. However, for so matter systems, where the
electron density varies considerably it does not work well and
the generalised gradient approximation (GGA) is better. For
chemisorbed molecules on solids the GGA oen gives
reason-able structural information but the adsorption energies can
depend strongly on the particular GGA functional.21 _{Hybrid}
functionals, which combine GGA with Hartree–Fock exact
exchange, give better results for covalently bonded systems and
have been used for studies of biomolecules on surfaces.22

A major limitation of the GGA and hybrid functionals is that
they are local and, therefore, do not account for non-local
eﬀects such as van der Waals (vdW) forces. For systems
con-taining somatter, vdW forces can be signicant and the GGA
is inadequate. It is, therefore, necessary to add a non-local
contribution to account for these interactions and various
schemes have been proposed for this. A more detailed overview
of these methods is given by Klimeˇs and Michaelides.23 _{The}
simplest approach is to add empirical dispersion terms to the
GGA energy,EGGA; the methods are generally referred to as
DFT-D methods.24,25_{The total energy is of the form}

E¼EGGA

X

A;B

CAB 6 rAB6;

where the CA,B6 coeﬃcients are treated as parameters and
depend on the atomic species A and B. However, the
CA,B6 coeﬃcients are constant throughout the simulation and
the values are not generally applicable to all bonding or
chemical environments. The DFT-D methods can be improved
by allowing theCA,B6 coeﬃcients to vary according to the
envi-ronment.26–28 _{A more general} _{rst-principles approach is to}
calculate the vdW forces using the charge density of the
system29 _{so that the exchange and correlation functional is}
given by

Exc¼Ex,GGA+Ec,LDA+Ec,nl (2)

where the rst term on the right is the exchange energy
described by the revPBE30_{form of the GGA, the second term is}
the local correlation energy using the LDA and the third term is
the non-local correlation energy, which is calculated from the
electronic charge density. This method is known as vdW-DF and

Fig. 1 Multiscale modelling of polymer–solid interfaces from the electronic structure level, through the atomistic level, to the mesoscopic coarse-grained level and beyond. Snapshots taken from ref. 18 and 19.

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

various modications to the exchange and non-local correlation
functionals have been proposed.31,32 _{The accuracy of these}
methods is oen compared using the S22 set of molecular
complexes,27,32,33 _{where the results of highly accurate CCSD}
methods are available. However, for extended systems, such as
hard–somatter interfaces, CCSD methods cannot be applied
and it is less clear which method is the best choice.

In summary, the balance between accuracy and
computa-tional eﬃciency means that DFT (with vdW) is arguably the best
approach for determining the adsorption behaviour of
mole-cules on solid surfaces and enables one to perform DFT
molecular dynamics studies of molecules on surfaces for a few
tens of picoseconds.22,34,35_{However, despite the computational}
eﬃciency of DFT, it is not possible to calculate macromolecules
on surfaces or small molecules for more than a few tens of
picoseconds. For larger systems and longer times classical
atomistic (usually molecular dynamics (MD) or Monte Carlo
(MC)) simulations are necessary. The accuracy of the classical
simulations relies on the quality of the atomistic forceelds.
Such simulations typically use simple pair potentials for the
interaction between polymer atoms, where the shape of the
potential can be controlledviaseveral adjustable parameters.
Standard forceelds, such as GROMOS36,37_{or OPLS,}38,39_{were}

tted to reproduce properties of somatter (e.g.homogeneous bulk systems) and are not designed to be used for so–hard matter interfaces. To describe accurately the interactions of an atom with the surface, it might be necessary to reparameterise these potentials or use diﬀerent types of functions.

For polymers it is convenient to divide the molecule into small
subunits, typically a monomer or sub-monomer, and calculate
the adsorption energies of these subunits separately. Potentials
are developed based on the interactions of these subunits and it
is assumed that the interactions of the diﬀerent subunits are
factorisable and uncorrelated. This technique is oen referred to
as the building-block approach and it has been used in studies of
bisphenol-A–polycarbonate on nickel,40_{organic molecules on}
rutile,41_{polypeptides on gold,}42,43_{and polystyrene on gold.}19_{The}
polycarbonate and polystyrene examples will be described in
more detail in the following sections.

There are several ways to parameterise forceelds based on
quantum mechanical calculations. One technique is to use a
combined DFT-MD/classical-MD approach to parameterise
analytical potentials via force matching.44–46 _{However, since}
DFT-MD calculations are expensive an alternative approach is to
use the results from static DFT calculations to optimise
inter-atomic potentials. The cheapest way to t pair potentials in
molecule–surface systems is to take an existing parameter set
and tweak the parameters so that they reproduce the properties
of a single (usually ground state) adsorption structure. However,
while this method may reproduce the energetics of the ground
state adsorption structure it is unlikely to represent accurately
the energetics of the variety of structures sampled during an MD
simulation. In order to obtain a realistic sampling of the
adsorption structures one must reproduce the potential energy
surface that includes intermediate energy congurations. The
issue of force eld representability was investigated using a
genetic algorithm to optimize Lennard-Jones parameters for a

large variety of adsorption structures.47,48 _{Other schemes use}
both the potential energy landscape and the atomic forces to
optimize numerical potentials but they have only been applied
to bulk solids.49–51_{More recently, an algorithm was developed to}
optimize accurate all-atom molecule–surface potentials that
reproduce a large set of DFT data.19,52_{The method is based on}
simulated annealing and the parameters of the nonbonded
interaction potential are chosen in order to minimize the target
cost function. The cost function is dened as the diﬀerence
between the quantum and classical molecule–surface
interac-tion energies, for many diﬀerent molecule–solid congurations,
i.e. diﬀerent distances from the surface, various adsorption
sites as well as diﬀerent molecule orientations. More details
about the method can be found elsewhere.52

The choice of the analytical form of the potential is also of importance. A commonly used potential in MD simulations is the 12–6 Lennard-Jones (LJ) pair potential,

VLJðrÞ ¼43

_{s}
r

12

s r

6

where3andsare adjustable parameters, and it enables the use of combination rules in MD simulations.

The GolP forceeld was developed to describe the
interac-tion between amino acids (proteins) and gold surfaces in
explicit water53_{and contains four terms, namely image charge}
interaction, chemisorption, van der Waals and conjugated
molecule interaction. The parameterisation of the
chemisorp-tion Lennard-Jones potential is based on DFT results and the
vdW interactions used MP2 data to parameterize 12–6
Lennard-Jones potentials. The GolP force eld has been applied to
studies of ubiquitin on gold nanoparticles.43

However, the Lennard-Jones potential may not be the optimal
choice for describing the interaction with a surface so other
potential forms may be more appropriate. For the interaction of
benzene and ethane on a gold surface19,52_{Lennard-Jones and}
Morse-type atomistic potentials were optimized to reproduce the
DFT adsorption energies as a function of distance from the
surface. The atomistic Morse potentials were of the form

VM(r)¼3[exp(2a(rr0))2exp(a(rr0))]

wherea,3andr0are all adjustable parameters for each type of atom pair combination. The potentials are shown in Fig. 2.

While both forms describe well the orientation dependence of benzene on the surface, it is clear that the Lennard-Jones potential overestimates the repulsion at close range whereas the Morse-type potential reproduces the adsorption energy over the entire range. Note also that a single set of Morse potential atom–atom pair parameters describe all diﬀerent adsorption sites, conformations and molecule–surface distances. However, it should be noted that the dependence of the DFT adsorption energies on distance is also uncertain, since it depends on the choice of exchange and correlation and van der Waals func-tionals. Other schemes, in particular those used in solid state physics, avoid the use of analytical forms for potentials, for example the Gaussian Approximation Potential (GAP) approach.51

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

Other DFT-based interface forceelds for polymers or large
molecules on surfaces have not used interatomic potentials but
instead have developed phenomenological potentials, such as a
wall-type potential with only az-dependence. This is typically
the case for coarse-grained models, for example a study of
bisphenol-A–polycarbonate on nickel40_{included 10}–_{4 }
Lennard-Jones potentials between the beads and the surface, which
correspond to integrated 12–6 Lennard-Jones interatomic
potentials. A similar method was used in the atomistic studies
of hydrated peptides on metal surfaces54_{and benzene and water}
on gold,55_{where the surface was represented by a}_{z}_{-dependent}
potential and repulsive or attractive potentials were added to
virtual sites in the molecule. In a study of polycarbonate on
silicon,56_{the adsorption of a polycarbonate monomer on the}
silicon surface was represented by attractive and repulsive
potentials and a distance-dependent angular potential on the
phenylene group. In addition surface site dependence was
introduced by adding repulsive cosine potentials on various
surface sites.

So far, the approaches described above are limited to rather
well-dened systems, with smooth, ideal surfaces and no
impurities and defects. Another important issue for classical
forceelds is reactivity, which is important for systems where
molecules may become chemisorbed on the surface. For these
systems it is important to use a forceeld that can describe the
diﬀerent bonding states of an atom. Several reactive forceelds
have been developed such as bond order potentials57,58_{and the}
ReaxFF forceeld.59

In summary, interface forceeld development has largely been ignored in classical studies of so–hard matter interfaces. However, as the demand for more quantitative and predictive capability increases the development of accurate interface force

elds will become an important issue.

### 3

### Classical atomistic simulations

As mentioned previously, atomistic simulations provide a
detailed all-atom description, as well as a quantitative
predic-tion of the properties of the hybrid multi-phase material. The
most common classical atomistic simulation methods that are
applied to hybrid polymer–solid systems are molecular
dynamics (MD) and Monte Carlo (MC). At the heart of MD
simulations is the numerical solution of Newton's classical
equations of motion, whereas the MC method is a numerical
scheme that involves random sampling of the
high-dimen-sional conguration space of a complex system. The main
limitation in the application of atomistic molecular dynamics
simulations to complex macromolecular materials is that it is
not possible to reach the long relaxation times of long-chain
polymers and, therefore, equilibration of such systems is diﬃ
-cult. MC methods allow a more eﬃcient sampling of the very
complex phase space of macromolecular materials by using
special MC moves that overcome strong energetic barriers.
However, it is not possible to study dynamics using standard
MC algorithms. More details about these methods can be found
in classic textbooks.60,61_{We should also note here that in many}
atomistic simulation studies united atom (UA) models, in which
hydrogens are lumped into carbons, are used. Such models, in
principle, belong to the family of coarse-grained models.
However, they are usually parameterized to reproduce the
properties of systems over a broad range of conditions and used
for quantitative studies. Therefore, we include them in the
family of atomistic models, but distinguish them from all-atom
(AA) models.

MD and MC simulations of polymer–solid interfacial
systems began to appear in the literature 2–3 decades ago.62–68
Most of the early work was concerned with very simple systems,
such as alkane chains using UA models, polymethylene,etc.,
and was restricted to short polymer chains. Xiaet al.used MD
simulations to study 1 and 2 nm thick n-hexadecane lms
adsorbed on a crystalline substrate.66 _{The alkane segmental}
density at the solid surface exhibited a regularly spaced
oscil-latory prole, with the amplitude of the density oscillations
decreasing with increasing distance from the solid surface and
extending about 2 nm into the lm. Winkler and Hentschke
studied the packing, orientation and local conformations of
polymethylene chains near adsorbing surfaces through
stochastic MD simulations.67_{Similarly, they observed an }
oscil-lating density prole, which returned to the bulk density around
1–2 nm from the surface. They also found that chains near the
surface were oriented almost parallel to the interface. A
combination of MC followed by energy minimisation was used
to study glassy atactic polypropylene on graphite65 _{and the}

attening of chains was found to extend over a region of 1.5Rg from the surface, where Rg is the unperturbed root mean

Fig. 2 DFT adsorption energies for benzene on the Au(111) surface in various orientations and on various surface sites.zis the distance between the centre of the benzene molecule and the top of the surface; T, H and B denote top, hollow and bridge sites, respectively andq¼0 (90) corresponds to a ﬂat (vertical) orientation. Symbols are the DFT data and lines are the classical adsorption energies using optimized (a) Lennard-Jones and (b) Morse potentials. Theﬁgure is taken from ref. 52.

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

squared radius of gyration of bulk polypropylene. This at-tening was due to reorientation of the chains rather than a change in chain conformation. Other studies have found that this attened region extends from the solid surface by a distance of about the end-to-end chain length, Re, for the specic model system.67,69

A hybrid MC–MD approach was developed for bulk polymer
systems, where MC algorithms are used to equilibrate rather
long chain systems, followed by multiple time step MD
simu-lations of the equilibrated structures.70–72 _{The MC method}
involved special chain connectivity-altering moves that allowed
a fast equilibration of long polymeric chains. This approach was
later applied to the study of various polyethylene–graphite (PE–
Gr) interfaces,69,73 _{using a UA model, with molecular lengths}
below and (slightly) above the entanglement molecular length.
The structure of the adsorbed layer on graphite was analyzed in
terms of the distribution of adsorbed segments in trains, loops,
and tails. The statistics of trains, loops and tails at the surface
has been calculated and found to be in reasonable agreement
with the predictions of Scheutjens–Fleer theory74,75_{for }
homo-polymer adsorption from solution, in the limit of zero solvent
concentration, in particular for the longer polymer chains.

The eﬀect of the solid surface on the dynamics of the
poly-mer has also been investigated. Diﬀusion constants can be
calculated based on the mean-square displacements of the
chain centers-of-mass or at the segmental level. For
poly-methylene it was observed that the mobility of the surface layer
is anisotropic; it is reduced in the direction normal to the
surface, due to the fact that particles are reected by the surface,
and it is increased, compared to bulk mobility, in the direction
parallel to the surface.67_{The latter is a result of using a smooth,}

at potential to represent the surface that results in a much
smaller friction factor, instead of a more realistic corrugated
surface.56,76 _{More recent studies of model polymer}–_{solid}
systems using an atomistic surface showed that the solid
surface causes signicantly slower dynamics compared to the
bulk dynamics.19,73,77_{This e}ﬀ_{ect only extends to a few nm from}
the surface. Furthermore, a detailed atomistic MD study of a
PE–Gr thick interfacial system,73_{of an unentangled chain (C}

78), showed that segmental dynamics of the adsorbed molecules perpendicular to the surface is quantitatively and qualitatively diﬀerent from that in the bulk and cannot be described by a constant diﬀusivity. It can, however, be accurately described using a macroscopic diﬀusion equation with a time-dependent diﬀusion coeﬃcient,D(t). In more detail, it was found that local segmental diﬀusivities (calculated via the mean square displacement of atoms) normal to the surface depend strongly on the thickness,d, of the layer next to the surface on which they lie at the beginning of diﬀusion: the closer the layer to the graphite plane, the slower the segmental mobility. In order for the segmental dynamics, normal to the surface, in the interface to become bulklike at all time instances, very large values ofd (equal to 6–7Rg for the C78 chains) containing only a small number of adsorbed atoms should be considered. It still remains to be seen whether this length scale depends on the polymer–solid interactions and on the molecular length of the polymeric chains. This is particularly important if we consider

that experimental studies with other polymer melt–solid surface
systems have proposed totally diﬀerent values for such a
distance, ranging from 3–4Rg78_{to 25}_{Rg}_{.}79

The glass-transition temperature,Tg, is also a very important
issue, and can be directly compared to experimental
measure-ments. The glass transition temperature can be calculated by
measuring the change in density as a function of temperature.
In a recent work Hudzinskyyet al.80_{calculated}_{T}

gfor supported polystyrene (PS)lms, using a UA model for PS, for the entire system as well as for three diﬀerent layers (substrate, middle, and surface) according to the density proles. They found that for the wholelm the average density-basedTgvalue remains almost constant for lms down to 2 nm thickness. For the middle layer itselfTgdoes not depend on the totallm thick-ness, while an increase of up to 70 K was measured for the substrate layer depending on the strength of attraction to the actual substrate. However, statistical errors became rather important for the very thinlms. The dynamics close to Tgis expected to be a non-universal phenomenon, governed by a complex interplay between adsorption, packing eﬀects and intramolecular rotation barriers.81

In the above studies the surface was represented by either a
simple phenomenological potential or by a standard
Lennard-Jones potential for the pair molecule atom–surface atom
interaction. However, as stated in the previous section,
quan-titative predictions of atomistic simulations depend on the
accuracy of the classical polymer–solid interaction potentials,
and properly designed interaction potentials that are
parame-terized based on quantum calculations are an important issue.
Borodinet al.82_{reported results from all-atom MD simulation}
studies of the interface between poly(ethylene oxide) and a
TiO2surface using a quantum-based forceeld. Johnston and
Harmandaris studied the structural and dynamical properties
of polystyrene conned between gold surfaces using an
inter-face forceeld that was developed using DFT calculations.19,52
The orientation, as well as the short time segmental dynamics,
for various vectors along the backbone and the side (phenyl)
group of the polymer chains was examined. Data showed a
strong tendency of both the backbone and phenyl groups to
orient parallel to the surface plane mainly for monomers that
belong to therst adsorption layer. In addition, the backbone
dynamics was found to be slower than the dynamics of the
phenyl groups, which are less constrained, whereas the
dynamics of both backbone and side groups is much slower
close to the Au surfaces.

Nowadays, with the large increase in computing power more
complex polymer–solid materials, such as nanopores, carbon
nanotubes (CNTs), polymer–graphene systems and
nano-particle composites, are being investigated using atomistic (AA
or UA) models.83–88 _{The e}ﬀ_{ect of surface geometries on the}
adsorption of the polymer is another relevant issue. For
instance, Barbieret al.83_{used fully atomistic MD simulations of}
a spherical silica nanoparticle of around 1.5 nm diameter in
polyethylene oxide (PEO). The results revealed a dense packing
ofattened PEO segments arranged in ordered shells around
the silica nanoparticle and the dynamics at the nanoparticle
surface was slower than the bulk dynamics, which is

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

qualitatively similar behaviour to a planar surface. Pandey and
Doxastakis87_{investigated in more detail the changes induced by}
curvature at length scales comparable to the polymer's Kuhn
length using silica nanoparticles of diameters ranging from 0.5–
3 nm in polyethylene as the model system and a new MC
sampling scheme that accelerated the polymer equilibration
close to the interface. It was shown that the surface
concen-tration of polymer chains is directly aﬀected by the increased
free energy cost of extending long sections of polymer chains
along the surface (trains), especially for small nanoparticles.
This results in shorter trains from more polymer chains at the
surface and a higher mass per unit area for highly curved
surfaces. Typical snapshots of PE–silica nanoparticles are
shown in Fig. 3. The MC results further support theoretical
studies89_{based on geometrical criteria that promote a decrease}
of the polymer bound layer thickness. They also highlight the
role of local rigidity on the scaling of the bound-layer with
particle size.

Another issue that has received a lot of attention is graing,
where chain ends are chemically attached to the surface. At
high graing densities the polymer has a brush-like structure
at the solid surface. Graed polyethylene chains with various
graing densities on graphite were studied using MC
simula-tions by Daoulaset al.90_{that resulted in slightly polydisperse}
systems. It was found that the local melt density in the region
closest to the interface is systematically higher than in the
bulk, exhibiting distinct local maxima due to polymer

adsorption, which is in agreement with non-graed polymer melts adsorbed on graphite. It was also seen that as the graing density increases, free chains are progressively expelled from the surface region, in agreement with scaling arguments and the predictions of lattice-based self-consistent mean-eld (SCF) theory.91

Furthermore, graing is an important aspect in controlling
the dispersion of nanoparticles in polymer matrices. Ndoro
et al.92_{presented a detailed atomistic study of hybrid systems of}
graed and ungraed spherical silica nanoparticles embedded
in polystyrene. They showed that the expected modication of
the polymer structure in the neighborhood of the particle is
stronger for higher graing densities and larger particle
diam-eters. In addition, the inltration of free PS chains into the
graed regime is reduced with increasing graing density, thus
making a NP with high graing density a poor choice for a
well-reinforced composite.

The study of polymers close to carbon nanotubes (CNTs) is
also a subject that has received a lot of attention during the last
few years.93–96 _{For example, Wei}94 _{has demonstrated that PE}
melt chains around a single SWCNT show a strong dependence
of the wrapping congurations on the radius and chirality of the
SWCNT. Furthermore, non-equilibrium properties, such shear
properties and thermal conductivity, have also been
investi-gated. Alaghemandi et al. used non-equilibrium MD
simula-tions to study the thermal conductivity of polyamide–CNT
composites and found that the addition of CNTs to polyamide
only increased the thermal conductivity moderately compared
to the pure polymer.97

### 4

### Coarse-grained simulations

Despite the advances in computation, atomistic models of hybrid polymer–solid materials are still restricted to relatively small systems with a simple monomer structure, such as poly-ethylene and unentangled polymer chains and nanocomposites with a single, small nanoparticle in a short-chain polymer matrix. To model larger and more complex polymer–solid interfacial systems one must reduce the chemical detail or degrees of freedom and model the hybrid system at a meso-scopic coarse-grained (CG) level. These methods are expected to be accurate for distances larger than a characteristic length, which is usually of the order of the Kuhn length.

Coarse-grained simulation approaches can be divided into two main categories based on whether their goal is: (a) to describe only qualitatively some generic (e.g. universal) features of complex hybrid systems (generic CG models) or (b) to quan-titativelypredict properties of the specic system under study (systematic CG models). Mesoscopic modeling approaches can be further decomposed on particle-based simulations andeld theoretical methods.

Generic coarse-grained models

This subsection begins with a short historical overview of simulation studies of hybrid polymer–solid materials using generic CG models. Therst coarse-grained simulation works

Fig. 3 Snapshots of model polyethylene–silica planar surfaces and nano-particles. Polymer molecules in contact with the surface are shown explicitly in black. Train segments belonging to diﬀerent chains are depicted for aﬂat surface.

Theﬁgure is taken from ref. 87.

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

of hybrid interfacial systems involved simple bead–spring or
lattice models. These models were found to be quite successful
in predicting the generic behaviour of polymer-solid materials.
Among therst coarse-grained simulation works of polymer–
solid interfacial systems are those of Bitsanis and
Hadziioan-nou who, through MD simulations of FENE chains,98,99_{}
inves-tigated the structure and microscopic dynamics in thinlms of
homopolymer melts conned between structureless, planar
solid walls. Yoon and co-workers68_{also studied the dynamics}
of short-chain systems near adsorbing surfaces through MD
simulations using typical bead–spring models. Manseld and
Theodorou carried out dynamic CG MC simulations on freely
jointed 20-bead model chain molecules in a cubic lattice in the
vicinity of solid walls.100 _{They evaluated the self-di}_{ﬀ}_{usion}
coeﬃcient of chains and its spatial dependence. In addition,
Aoyagiet al.101 _{carried out MD simulations of polymer melts}
conned between walls with a bead–spring model. The eﬀect
of the interface on the relaxation of polymer chains was
studied by analyzing the time autocorrelation functions of the
normal modes as a function of distance from the wall. The
dynamics of polymeric chains conned between nonadsorbing
solid surfaces has also been studied through MC calculations
using the bond uctuation model. MC data showed that for
such systems segmental mobility is enhanced as the lm
thickness is decreased, but the overall chain dynamics remains
unaltered.102

In all the above cases polymer dynamics was qualitatively studied by calculating the mean-square center-of-mass displacement of polymer segments (beads) as a function of simulation time. The latter quantity showed a dramatic reduc-tion in chain mobility near strongly adsorbing walls over several layers, but an enhancement near weakly adsorbing walls, mainly as a result of a decrease in polymer segmental density. Strong segment–wall attractive interactions were also seen to appreciably prolong relaxation times, in comparison to the bulk. These data are in general qualitative agreement with the behavior of more detailed atomistic simulation models, dis-cussed in the previous section.

The dynamics ofuid polymers in conned geometries is
also a topic studied extensively in the past through generic CG
models.103–107_{The main questions in this topic are related to the}
dependence of the velocity prole, and the slip length (i.e.
the proportionality coeﬃcient between the slip velocity and the
shear rate), on the boundary conditions at the liquid–solid
interface. Most works in the literature concern atomically
smooth, homogeneous surfaces and the slip length has been
calculated for various systems.107,108 _{More recently the slip in}
thin polymer lms conned by either at or periodically
corrugated surfaces was investigated by simple FENE models.109
It was shown that the eﬀective slip length for corrugated
surfaces depends on the wavelength of the corrugation: for
wavelengths larger than the radius of gyration of polymer
chains, the eﬀective slip length decays monotonically with
increasing corrugation amplitude, and the data can be
described accurately by the numerical solution of the Stokes
equation with constant and rate-dependent local slip length. In
contrast, for corrugation wavelengths comparable to the radius

of gyration, the continuum predictions overestimate the eﬀ
ec-tive slip length obtained from molecular dynamics simulations.
From the above discussion it is clear that simple CG models
can be successfully used in order to study and predict generic
(e.g. universal) properties of polymer–solid hybrid systems.
Their main advantages are related with their simplicity (i.e.
simple form of CG bead–bead interactions) and their
compu-tational eﬃciency, compared to detailed atomistic models.
Because of this such models are still used to predict the generic
behavior of complex hybrid systems. For example, in a recent
work De Virgiliset al.110_{used a bead}_{–}_{spring model to study a}
polymer melt at a surface for various degrees of adhesion. They
showed that the average length of trains and loops does not
depend signicantly on the adsorption strength, whereas the
number of loops and trains slightly decreases with increasing
adhesion. The dynamics of the adsorbed layer was found to
follow a slightly non-Arrhenius behavior with the adsorption
potential.

All the above works concerned polymer chains in contact
with (or conned between) planar solid surfaces. Other topics in
which generic CG models can be very useful is modeling the
behavior of complex polymer-graed surfaces and polymer
nanocomposites that cannot be studied with all-atom models.
The latter topic, in particular, is a subject in its own right that
deserves an extended discussion; see for example the review by
Zenget al.17_{Here we do not wish to discuss this issue in detail}
but we feel that it will be useful to include a few examples, since
they are closely related to polymer–solid interfacial systems. For
instance, a system of model polymer chains attached to aat
surface (polymer brush) was studied by the pioneering work of
Grest111_{through MD and MC simulations using a simple bead}–
spring model. Both MD and MC studies showed layering of
monomers close to the surface, in agreement with a system of
polymer chains in contact with solid surfaces. In addition, the
simulation data are in reasonable agreement with data from
more detailed atomistic simulations discussed in the previous
section.90

During the last decade CG studies of more complex graed polymer–solid systems were reported. Pakula and Klos112,113 applied lattice MC simulations, with a cooperative motion algorithm to a system of linear chains end-graed to a spherical surface. Good solvent conditions were considered and the monomer concentration proles were found to change from concave to convex with increasing nanoparticle radius. For small surface coverage and for small nanoparticles with a high curvature, polymer conformations in which a chain can wrap around the nanoparticle were also observed. Kalb et al.114 further analyzed the eﬀect of surface coverage and curvature of spherical graed nanoparticles for an entangled system.

The computational eﬃciency of simple bead–spring models
allows them to be used to study systems of high molecular
weight, such as entangled polymer chains close to SWCNT that
cannot be studied in full atomistic detail. In such a work
Kar-atrantoset al.115_{showed that in the presence of a SWCNT (with}
or without attractive interactions), the network of topological
constraints (entanglements) is modied,i.e.the contour length
of the primitive path increases indicating more entanglements.

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

Moreover, concerning the dynamics of polymer chains, large
heterogeneity was found due to the polymers in contact with the
SWCNT. Furthermore, Smith and co-workers76 _{used a simple}
bead–spring model to study viscoelastic properties of various
polymer–nanoparticle systems with diﬀerent nanoparticle–
polymer interactions. They showed that viscoelastic properties
of the polymer matrix were strongly perturbed by the NPs and
depended upon the nature of the nanoparticle–polymer
inter-actions. Standard bead–spring models can also be used to
provide a qualitative picture about the nature of the direct, or
mediated, eﬀective interaction between nanoparticles
embedded in a polymer matrix.116 _{More recently Cordeiro}
et al.117_{investigated the interaction (mutual repulsion) between}
two graed surfaces. They have shown that repulsive surfaces
made chains to attain more extended conformations, than
chains adsorbed onto attractive surfaces.

Furthermore, the glass transition of polymers near
inter-faces, and of polymer nanocomposites, has been studied using
generic CG approaches based on percolation models. In such
models the glass transition is explained as a dynamical
proce-dure.118–122_{In more detail, Long and Lequeux}_{rst proposed that}
a material exhibits a macroscopic glass transition when small
slowly relaxing regions percolate through the sample.118 _{They}
applied their model to general van der Waals liquids in bulk
and in thinlms. Later Kropkaet al.used the percolation model
to examine the changes inTgfor polymer nanocomposites and
their equivalence for thinlms.120,121_{More recently Lipson and}
Milner applied the percolation model for a polymer thinlm.
They show that, as predicted by the model, a free surface
reduces the number of paths that connect a site, near to the
surface, to percolating clusters, thus lowering the Tg of the
polymer. However, the magnitude of this eﬀect is not enough to
account for the lowering ofTgobserved experimentally, showing
that other mechanisms may also contribute to the complex
glass transition behavior.122

Hybrid polymer–solid nanostructured systems have also
been studied using a family of compressible free energy
coarse-grained models based on traditional integral equation theories,
such as the microscopic Polymer Reference Integration Site
Model (PRISM).123_{In these models, chains are represented as}
bonded sites that interact via pair decomposable site–site
potentials, composed of a repulsive branch (usually hard core)
and longer range attractive interactions. The advantage of such
models is that they allow a qualitative study of the structure and
the phase diagram of more realistic model nanocomposite
systems with many nanoparticles. In more detail, Schweizer and
co-workers124–126_{extended the PRISM theory to study polymer}
nanocomposites, by incorporating specic polymer–
nano-particle and nanonano-particle–nanoparticle contributions. Their
work showed that depending on the range of intermolecular
interactions, the particle–particle potential of mean force can
show contact aggregation, steric stabilization, local and longer
range (mediated by the environment) bridging attraction. These
data could help to designllers in polymer melts with specic
thermodynamic stability and miscibility.

Following a similar methodology Frischknechtet al.127_{have}
studied the eﬀect of well dispersed nanoparticles on the

equilibrium chain congurations using a coarse-grained self-consistent polymer reference interaction site model (SC/PRISM). They observed an increase of polymer chain dimensions with increasing nanoparticle volume fraction for small nanoparticles with radius below the chain dimensions. This chain expansion eﬀect was attributed to the attractive interaction between the monomers and the nanoparticles, as well as to the excluded volume taken up by the nanoparticles; both phenomena result in making the nanoparticles behave like a good solvent.

We should note here that all the above models oﬀer a quite successful qualitative prediction of the structure and dynamics of generic polymer–solid interfacial systems, but lack a link to specic systems. In many cases a mapping of the model parameters onto data taken either from more detailed atomistic simulations or experiments provides also quantitative agree-ment with specic polymer–solid nanostructured systems.124 However, a rigorous linking with microscopic all-atom model systems requires systematic CG models developed directly from the chemistry.

Systematic coarse-grained models

Systematic coarse-grained models are developed based on
atomistic models and aim at retaining the essential chemistry of
the system. The main idea behind coarse-graining is to lump
groups of chemically connected atoms into“superatoms”and
derive the eﬀective CG interaction potential by taking into
account the atomistic details of the particular polymer. CG
models can diﬀer in the degree of coarse-graining (the number of
real atoms that correspond to one“superatom”) as well as in the
way the eﬀective CG potentials are derived. For structure-based
CG models, a direct link to the chemistry is achieved through
structurally dened bonded and nonbonded eﬀective CG
potentials derived from the atomistic model.128–130_{Such models}
have been applied with success to study quantitatively the
structure, conformations and the thermodynamics of various
bulk polymer systems. However, the direct usage of such CG
models to describe the dynamics of complex systems is a more
subtle issue. The reason is that due to the reduced degrees of
freedom in the CG description, the friction between the CG beads
is signicantly reduced compared to what it would be if the
monomers were represented in full atomistic detail. Therefore,
the time scale in the CG description does not correspond to the
one of the microscopic (underlying) chemical system. To
over-come this limitation diﬀerent methods are followed in the
literature that are related either to an appropriate
parameteri-zation of the CG time scale130–132_{or to the involvement of the}
friction forces in the equations of motion.133,134_{Following these}
approachesquantitativeinformation about the dynamics of bulk
polymer systems can be also provided from the CG models. An
additional advantage of systematic CG models, in which each CG
“superatom”represents about O(10) atoms, is that detailed
all-atom congurations of the model CG systems can be obtained
through a back-mapping algorithm.128,135

The extension of systematic CG models to polymer–solid interfacial systems is a challenging research area because of extra complexities due to the presence of interfaces. Therefore,

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

only a few systematic CG studies have been applied to polymer–
solid multi-phase systems. For example, the interaction of
liquid polycarbonate near a nickel surface was studied by
directly connectingab initiodensity functional calculations to
coarse-grained molecular dynamics simulations.40,136 _{Density}
functional calculations of the adsorption of polymer fragments
on the surface were used to parameterise the surface potentials.
Based on the DFT calculations it was concluded that only the
benzene subunits at the chain ends had the conformational
freedom and a strong enough adsorption to adhere to the nickel
surface, resulting in a polymer brush structure. They found that
the surface only inuenced the structural properties up to 2Rg
from the surface, whereRgz1.9 nm for 10mer BPA-PC. These
results are in agreement with the data from the more detailed
atomistic simulations presented in the previous section. This
model was used in subsequent investigations of chain end
modication137_{and shear properties.}138,139 _{A similar approach}
was used to study BPA-PC on a Si(001)-(2 1) surface, which
found similar structural properties at the surface.56

It should be noted that the above methodology that
param-eterises the surface potentials using ground-state
zero-temper-atureab initiocalculations does not properly describe entropy.
Thus, this method is expected to be valid only for strong
poly-mer–solid interaction energies, i.e.chemisorption, while it is
not a good approximation for weakly interacting polymer–solid
systems that are dominated by van der Waals interactions. In
the latter case, entropy should be taken properly into account.
This could be partially achieved by using DFT-MD
simula-tions140_{to obtain an entropy-averaged adsorption energy for the}
polymer fragment. However, such methods can only be used for
very small molecules; thus the entropic contribution is not
really representative of a realistic polymer chain. Alternatively,
entropy eﬀects could be included by using atomistic MD
simulations of the polymer chain on the surface to parameterize
the CG interface potentials. Of course, to retain chemical
accuracy the atomistic interface force eld should itself be
parameterized using DFT calculations.

Overall, the need for direct quantitative studies of complex realistic polymer–solid interfacial systems with high molecular weight makes the development of systematic CG models for polymer–solid hybrid systems a very intense research area. Through the above discussion it is also clear that this is also a very challenging area, since it directly involves linking between quantum, microscopic (atomistic) and mesoscopic (coarse-grained) simulations.

### 5

### Field theoretical models

An alternative family of mesoscopic simulation approaches
used to describe polymer–solid complex systems are eld
theoretical based methodologies.141 _{Field theoretical }
simula-tions for polymers on solid surfaces began with the seminal
Scheutjens–Fleer self-consistenteld theory (SCFT),74,75_{which}
analyzed the polymer chain conformations of a polymer
solu-tion close to a solid substrate and predicted the corresponding
scaling laws. As described in the previous section, their
predictions are in good agreement with particle-based

molecular simulations of a polymer melt. These methods were
extended to describe in more detail polymer–solid interfacial
systems. For example, Daoulas et al.142 _{showed that }
self-consistent eld calculations with the worm-like chain model
that incorporates local stiﬀness provide a better description of
the adsorption of PE molecules. Trombly and Ganesan143
studied the curvature eﬀects of polymer-graed nanoparticles
in a polymer melt. The interpenetration width between graed
and free chains was studied as a function of the curvature of the
surface, the graing density, and the relative molecular weights
of the graed and free chains. A greater tendency for
inter-penetration of free chains into the graed chains regime with
increasing surface coverage was found to be due to entropy.

During the last few years several diﬀerent eld theoretical
approaches, using methods that go beyond the mean eld
approximation, have appeared in the literature.144–149 _{These}
approaches are usually hybrid simulation methods such as (a) a
scheme that combines SCFT for polymers with classical density
functional theory for particles,144_{(b) particle-}_{eld simulations in}
which the coordinates and chemical potentialeld variables are
updated simultaneously,146_{and (c) MC particle-based approaches}
within the quasi-instantaneouseld approximation where the
interaction of a monomer with its surroundings is expressed
through aeld that is frequently updated from the instantaneous
positions of the particles.145,150,151_{All the above approaches are}
very promising for complex polymer–solid interfacial systems
due to their strong computational eﬃciency. For instance,
The-odorou and co-workers152 _{applied a Monte Carlo sampling}
formalism to investigate the structure of a polymer matrixlled
with tightly cross-linked polymer nanoparticles. As expected both
the density and the local structure of the polymer matrix in the
vicinity of the nanoparticles are found to be diﬀerent from those
of the corresponding bulk, in accordance with the data of the
more detailed atomistic and particle CG simulations. In addition,
they found that the dispersion of many nanoparticles in the
polymeric matrix leads to extension of the chains when their size
is similar to the radius of the dispersed particles.

Overall, the above models provide eﬃcient computational approaches for accessing the behaviour of complex polymer– solid hybrid systems, at least for length scales longer than the Kuhn segment. Their direct relation to the chemistry at the nanometer scale, which is particularly important for nano-structured materials, is a very challenging topic. We should also note that the studies discussed above are only a small portion of the eld theoretical simulation approaches reported in the literature. A complete review of thiseld is far beyond the scope of the present article and we recommend some excellent reviews that have appeared in the literature in the last few years.123,153–156

### 6

### Outlook

The study of hybrid polymer–solid interfacial materials at the molecular level through simulation approaches is a very intense research area that has mainly addressed: (a) the deviation of various polymer melt properties from their bulk values (i.e. structural, conformational, dynamical, etc.), induced by the presence of the interface, and (b) the extent of these changes

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

from the interface. The current level of fundamental knowledge shows clearly that the length of the interface depends on the actual property under consideration.

In particular the main ndings for model polymer–solid interfaces, where the polymer chains are physisorbed onto the solid surfaces, are the following: (a) the segmental density of a polymer melt close to the interface shows an oscillating density prole with a clear maximum very close to the surface, which reaches the bulk density around 2–3 nm from the surface. This length scale appears to be independent of the monomer struc-ture (chemistry) as well as the length of the polymer chains. (b) Conformations of polymer chains are clearly perturbed close to the surface, i.e. chains near the surface are oriented almost parallel to the interface. The polymer conformations are

modi-ed over a region up to around 2Rgfrom the surface. This length scale seems also to be independent of the polymer chemistry for the systems studied till now. (c) Orientational dynamics of the polymer chain at the segmental level, quantied usually by the decorrelation of a vector along the monomer, is slower near the solid substrate than in the bulk. The extent of the slower dynamics is up to a few (2–4) nm from the solid substrate. It further seems not to be strongly dependent on molecular length, as should be expected for segmental dynamics.

Despite the many advances that have been made in the modeling of polymer–solid hybrid systems, there are still many open questions and challenges, both from the view of funda-mental physics and the development of simulation approaches. We have listed the following open issues that we believe are among the still important and relevant questions.

Glass transition temperature

Despite the large number of experimental studies in the
litera-ture, the eﬀect of the substrate onTgis still under debate. This
is directly related to experimental diﬃculties in studying very
thinlms, and measuringTgas a function of distance from the
surface, rather than an average value over the whole lm.
Furthermore, there are additional complexities if someone
compares the dynamicvs.calorimetricTgand clear indications
of dynamic heterogeneities close to the surface have been
reported.157_{To understand this phenomenon further, detailed}
investigations of the distribution of segmental relaxation times
at the solid surfaces compared to the bulk would be very useful.

Fluid dynamics at the interface

The eﬀect of the surface on the polymer melt dynamics at the
molecular level is also a very important issue. It is directly
involved in studies related to slip phenomena and systems
under non-equilibrium conditions. Even more, it has a strong
inuence on the rheological and linear viscoelastic properties of
the hybrid material.1,6_{To clarify such issues, detailed studies of}
the chain, as well as the segmental, dynamics for various
specic polymer–solid systems are needed.

Molecular weight dependence of properties

Several fundamental questions of polymer physics are related with the molecular weight dependence of the dynamics of

polymer chains in contact with the surface.4_{For instance, how}
well do the Rouse and the reptation exponents of the diﬀusion
coeﬃcient describe the dynamics of polymeric chains in contact
with the surface? Are there universal power laws in accordance
with the dynamics of bulk systems or do the exponents depend
on the actual strength of the polymer–solid interaction? Is the
network of entanglements at the interface very diﬀerent to the
bulk, unperturbed one? The answer to these questions will
further help theoretical approaches aiming at the prediction of
the dynamics and the rheology of hybrid polymer–solid
systems.

Geometric eﬀects

The detailed surface properties could have a pronounced eﬀect on the structure and dynamics of the polymer near the surface. More studies are needed to address issues such as surface roughness and curvature. These will aﬀect the ordering and the packing of the polymer as well as the friction at the surface. Such issues are further related to systems with more complex geometries of the solid phases, such as nanopores and nano-particles with non-spherical geometry. Therefore, direct inves-tigation, at the molecular level, of the inuence of the degree, the specic type of corrugation, and of curvature on the prop-erties of atoms at the interface is critical.

Fluctuations at the interface

Most of the current simulation approaches do not analyze in detail the thermaluctuations at the interface. For example, the variability in the strength of adsorption for atoms/mono-mers in contact with a solid substrate is usually not discussed and average quantities are reported. However such issues might be important in the eﬀective interaction between nanoparticles immersed in a polymer melt as well as the phase diagram of the hybrid material. Detailed investigation of the statistics of structural and dynamical quantities at the interface will be helpful to clarify the importance of such issues.

Collective phenomena in polymer-based nanocomposites

A major challenge in the simulations of polymer nano-composites is to model more realistic systems with many nanoparticles. This will allow, at the molecular level, collective phenomena related to the eﬀective interaction between nano-particles to be studied, as a function of distance between them, and as a function of their concentration. This is particularly important if we consider that experimentally the dispersion of NPs is a rather problematic issue.15

Concerning the challenges related to the development of simulation methodologies we consider the required work in the following directions. First, there is a clear need to develop new and improved simulation algorithms in specic length-time scales. Second, it is even more important to develop systematic approaches to link methods over a wide range of length and time scales. In more detail, some of the major challenges in this

eld are the following:

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a

1. Systematic hierarchical approaches that link quantum
(DFT) to atomistic and atomistic to CG scale for polymer–solid
systems are still in their infancy. To link DFT to atomistic
simulations there are certain issues related to the rigorous
matching ofab initiodata (forces and energies) that allow the
correct description of structure and entropy. The specic
inter-actions close to the substrate might also involve the formation
and breaking of chemical bonds, which would require reactive
MD methods. For linking the atomistic to CG simulations an
accurate estimation of the non-bonded CG bead–surface eﬀ
ec-tive free energy and correct incorporation of the local polymer
rigidity in the CG model are crucial. Of analogous importance is
also the direct linking between atomistic (or CG) models to
continuum ones.17_{Furthermore, the quantitative prediction of}
dynamics of polymer–solid systemsviasimulation
methodolo-gies is an important issue for all approaches. In order to correctly
predict the dynamics in the all-atom model the classical force

elds should accurately describe the friction at the interface. In this case standard potentials based on the parameterization of DFT data (zero temperature) might not be enough. In order to correctly predict the dynamics with the CG models, the methods currently used to correct the CG time scale in bulk systems, based either on a post processing time rescaling step orviathe inclu-sion of friction forces in the equations of motion, should be extended and/or new methodologies should be developed.

2. Clearly there is a need for simulation methodologies that
span diﬀerent levels of description simultaneously. The
develop-ment of such methods is a very activeeld with several methods
developed for bulk systems going from quantum mechanics to
atomistic,158,159_{from atomistic to CG}160_{and from atomistic or CG}
models to continuum ones.17_{The extension of these approaches to}
hybrid systems could combine the advantages of all-atom models
close to the interface and CG or continuum far away from it.

3. Equilibration issues are also an important topic in the modeling of complex polymer–solid systems with long poly-meric chains. Indeed the equilibration of high molecular weight entangled chains close to the substrate or to nanoparticles might be a diﬃcult task that requires more time than is computationally feasible. The combination of systematic CG techniques and advanced MC algorithms seems to be an attractive direction for overcoming such problems.

In summary, the development of hierarchical or simultaneous multiscale simulation methods for complex systems is a very challenging topic in computer simulation and modeling, with a major goal being the direct quantitative comparison between experiments and simulations. To achieve this, new mathematical and computational concepts will be required. These develop-ments are crucial in order to accomplish the longstanding goal of material design and predict the structure–property relationships of complex materials at the molecular level.

### Acknowledgements

We would like to thank Thomas Vilgis, Vakhtang Rostiashvili and Kostas Daoulas for valuable discussions. Funding for Karen Johnston was provided by the German research foundation grant SPP-1369.

### References

1 J. Koo,Polymer Nanocomposites: Processing, Characterization, and Applications, McGraw-Hill, 2006.

2 A. J. Kinloch,Adhesion and adhesives: science and technology, Chapman and Hall, New York, 1987.

3 H. Kim, A. A. Abdala and C. W. Macosko,Macromolecules, 2010,43, 65156530.

4 M. Doi and S. F. Edwards,The Theory of Polymer Dynamics, Clarendon Press, Oxford, England, 1986.

5 H. Hu and S. Granick,Science, 1992,258, 1339.

6 G. Tsagaropoulos and A. Eisenberg,Macromolecules, 1995, 28, 6067.

7 S. Granick, S. K. Kumar, E. J. Amis, M. Antonietti, A. C. Balazs, A. K. Chakraborty, G. S. Grest, C. Hawker, P. Janmey, E. J. Kramer, R. Nuzzo, T. P. Russell and C. R. Sanya,J. Polym. Sci., Part B: Polym. Phys., 2003,41, 2755.

8 R. D. Priestley, C. J. Ellison, L. J. Broadbelt and J. M. Torkelson,Science, 2005,309, 456.

9 J. A. Forrest, K. Dalnoki-Veress, J. R. Stevens and J. R. Dutcher,Phys. Rev. Lett., 1996,77, 2002.

10 M. Y. Efremov, E. A. Olson, M. Zhang, Z. Zhang and L. H. Allen,Phys. Rev. Lett., 2003,91, 085703.

11 A. Serghei, H. Huth, C. Schick and F. Kremer, Macromolecules, 2008,41, 3636.

12 M. Tress, M. Erber, E. U. Mapesa, H. Huth, J. Mueller, A. Serghei, C. Schick, K.-J. Eichhorn, B. Voit and F. Kremer,Macromolecules, 2010,43, 9937.

13 E. P. Giannelis, R. Krishnamoorti and E. Manias, Adv. Polym. Sci., 1999,138, 107.

14 S. Anastasiadis, K. Karatasos, G. Vlachos, E. Manias and E. P. Giannelis,Phys. Rev. Lett., 2000,84, 915.

15 S. S. Ray and M. Okamoto,Prog. Polym. Sci., 2003,28, 1539– 1641.

16 M. R. Bockstaller, R. A. Mickiewicz and E. Thomas, Adv. Mater., 2005,17, 1331–1349.

17 Q. H. Zeng, A. B. Yua and G. Q. Lu,Prog. Polym. Sci., 2008, 33, 191–269.

18 R. Pek¨oz, K. Johnston and D. Donadio,J. Phys. Chem. C, 2012,116, 20409.

19 K. Johnston and V. Harmandaris,SoMatter, 2012,8, 6320– 6332.

20 R. M. Martin,Electronic structure: basic theory and practical methods, Cambridge University Press, 2004.

21 K. Johnston, A. Gulans, T. Verho and M. J. Puska,Phys. Rev. B: Condens. Matter Mater. Phys., 2010,81, 235428.

22 A. Rimola, M. Aschi, R. Orlando and P. Ugliengo, J. Am. Chem. Soc., 2012,134, 10899.

23 J. Klimeˇs and A. Michaelides, J. Chem. Phys., 2012, 137, 120901.

24 S. Grimme,J. Comput. Chem., 2004,25, 1463.

25 K. Tonigold and A. Gross,J. Chem. Phys., 2010,132, 224701. 26 A. D. Becke and E. R. Johnson,J. Chem. Phys., 2007,127,

154108.

27 A. Tkatchenko and M. Scheﬄer,Phys. Rev. Lett., 2009,102, 073005.

Open Access Article. Published on 20 May 2013. Downloaded on 29/08/2013 16:19:43.

This article is licensed under a